Energy Procedia 6 (2011) 1–5
Available online at www.sciencedirect.com
Investigation of Emitter Homogeneity on Laser Doped Emitters
Sven Germershausena*, Lars Bartholomäusa, Ulf Seidela, Norbert Hanischa, Anja Schieferdeckera, Karl Heinz Küstersa, Martin Kittlerb, Mawuli Ametowoblac,
Florian Einselec, Gerald Dallmannd aConergy SolarModule GmbH & Co.KG, Conergy Str. 8, 15236 Frankfurt (Oder), Germany
bLeibniz Institute for Innovative Microelectronics (IHP), Im Technologiepark 25, 15236 Frankfurt (Oder), Germany cManz Automation AG, Steigäckerstr. 5, 72768 Reutlingen, Germany
dSGS Institut Fresenius GmbH, Königsbrücker Landstr. 161, 01109 Dresden, Germany
The selective emitter formation by laser doping is a well known process to increase the efficiency of silicon solar cells , . For the characterization of laser doped emitters, SIMS (Secondary Ion Mass Spectroscopy) and ECV (Electrochemical Capacitance Voltage Measurement) techniques are used to analyze the emitter profile . It is very difficult to get acceptable result by SIMS on a textured surface, so only ECV can be used. It has been shown, that a charge carrier depth profile can be measured on a homogeneous emitter only by ECV. The use of laser doping results in a non-homogeneous emitter. We have shown that the emitter depth is not just a function of the pulse power, but in addition of the surface structure of the wafer. The texture seems responsible for a strong variability in the doping profile. It has been shown, that the ECV measurement is not applicable to characterize the emitter depth on laser doped areas, because of the microscopic inhomogeneities in the emitter on the macroscopic measurement area. The real emitter profiles are to complex to be characterized by SIMS or ECV. We have shown that the variation in the emitter profile is resulting from the texture in the laser-doped regions.
Keywords: Laser doping, selective emitter, doping profile
* Corresponding author. Tel.: +4933552113287 E-mail address: [email protected]
1876–6102 © 2011 Published by Elsevier Ltd. Selection and/or peer-review under responsibility of SiliconPV 2011. doi:10.1016/j.egypro.2011.06.129
Energy Procedia 8 (2011) 232–237
Open access under CC BY-NC-ND license.
© 2011 Published by Elsevier Ltd. Selection and/or peer-review under responsibility of SiliconPV 2011
Open access under CC BY-NC-ND license.
Sven Germershausen et al. / Energy Procedia 8 (2011) 232–237 233
SIMS is a standard measurement method to get carrier depth profiles. It is difficult to get a stable sputter rate on heavy structured surfaces. For that reason it is only possible to get significant results on planar surfaces. For industrial inline spray diffusion, the wetting process of the wafer depends on the surface energy. Emitter formation on different surfaces varies . Results from textured and planar surfaces are not comparable. Therefore SIMS on textured surfaces is not applicable.
Using ECV it is possible to measure on textured surfaces. The surface will be etched, and the capacitance is measured. By the alternation of etching and measuring, a charge carrier depth profile will be obtained. The accuracy of this method depends on how accurately the size of the area with the electrolyte in contact is known . Another advantage is that ECV measures only the active phosphorus concentration. Based on the depth profile, the sheet resistance can be calculated.
( ) 1
⎞ ⎜⎜ ⎝
⎛ ∫= dzznR d
S σ (1)
To investigate a homogenous standard emitter, this method can be used, because there are no strong
lateral differences in the depth (Fig. 2a). When the emitter in the survey area is highly inhomogeneous, however, then this method is not suitable to describe the depth profile (Fig.3b; 4b).
d junction depth
σ resistance of the layer
n density of free charge carriers
2.1. Investigation of the homogeneity of standard in-line emitters
On industrial standard mono crystalline wafers (resistivity: 1.5-3 Ohm*cm) with an acidic texture, a 85 Ohm/sq and a 115 Ohm/sq emitter with standard production equipment was created. After removing the PSG (Phosphorus Silicate Glass), the carrier depth profile was measured with ECV (3 measurements on the 85 Ohm/sq and one on the 115 Ohm/sq wafer) and the sheet resistance was measured with a capacitive method. Beside the ECV measurement, we cracked the wafer and decorate the emitter with an etching mixture, so that only the n-doped area is etched which is detectable with the SEM (scanning electron microscopy). After measuring the emitter depth with the SEM, both results were compared.
On standard multi crystalline wafers (resistivity: 1-1.5 Ohm*cm) a 115 Ohm/sq emitter with the same standard production equipment was created. The homogeneity of the emitter has been also investigated by emitter decoration. However, no ECV profiles were measured.
234 Sven Germershausen et al. / Energy Procedia 8 (2011) 232–237
2.2. Investigation of the homogeneity of laser-doped emitters
In a second step, we created a 115 Ohm/sq emitter on mono crystalline silicon (standard acidic texture) and did not remove the PSG layer. With the help of a q-switched, frequency doubled solid state laser (532 nm), areas on the wafer with a lower sheet resistance were produced by the irradiation of the PSG with the laser (patented IPE-procedure ; Institute for Physical Electronics of the University Stuttgart; Fig.1a, b). The emitter depth on these different doped regions was measured with ECV and the sheet resistance was calculated. The sheet resistance was also determined by a capacitive method. All of these test areas were decorated to make the emitter visible. The results have been compared.
Fig. 1 (a) Schematic of the laser-assisted doping process with phosphorus silicate glass as source (01 Pulsed laser beam, elliptical beam profile; 02 PSG-layer; 03 Diffusion of phosphorus in the Silicon melt; 04 highly doped contact region) (b) Sheet resistance vs. pulse energy density (stable repetition rate and scan velocity; min = 3 J/cm², max = 4.8 J/cm²) 
3. Results and Discussion
3.1. Homogeneity of standard in-line emitters In Fig 2a, a decorated 115 Ohm/sq emitter is shown. The generated spray diffusion emitter is very
homogenous. Comparing SEM measurement (Fig.2a) with the ECV profile (Fig.2b), a difference in thickness has
been found. These measurement variations are comparable to all measurement areas on the wafer. ECV shows approximately, how deep the emitter could be (Tab.1). This method can therefore be used for homogeneous emitters.
Table I. Comparison between the measured emitter depth with ECV and the measurement with SEM (mono crystalline silicon) for an 85 Ohm/sq emitter (CM = capacitive measurement)
Mean of sheet resistance (Ohm/sq), CM 85
Mean of sheet resistance (Ohm/sq), ECV 91
ECV emitter depth (4E16 1/cm³; range, mean) [nm] 165-200 (181)
SEM emitter depth (range, mean) [nm] 95-183 (145)
Sven Germershausen et al. / Energy Procedia 8 (2011) 232–237 235
Fig. 2 (a) Homogenous emitter 115 Ohm/sq (decorated) on mono crystalline silicon, created by inline diffusion; (b) Emitter depth profile (ECV measurement, 115 Ohm/sq)
Multi crystalline material has a lot of lattice defects in the crystal . This can lead to inhomogeneities in the emitter (Fig. 3b). ECV measurements are, due to the large measured area, only partly suitable to characterize such an emitter. Microscopic differences in the emitter thickness could not be observed by using this method (compare Fig. 3a and 3b).
Fig. 3 (a) Relatively homogenous emitter 115 Ohm/sq (decorated) on multi crystalline silicon, created by inline diffusion, (b) inhomogeneous emitter 115 Ohm/sq of multi crystalline silicon, caused by crystal defects
3.2. Homogeneity of laser-doped emitters
The target of selective emitter processing should be a sheet resistance below 50 Ohm/sq to get an acceptable contact resistance. To obtain these values, the silicon surface has to be melted for a specific time by irradiation with a specific energy density (Fig. 1b).
The investigations show that the emitter is inhomogeneous in the laser-doped region (Fig. 4a-d, 5a). This is caused by the different coupling conditions for the laser radiation and the differences in the heat conduction. Both are influenced by the texture structures. Also the influence of heat conduction is a dominant factor.
By increasing laser power the homogeneity of the emitter is reduced (Fig. 4a-c) . Overheating and thus a longer melt time could lead to the formation of a deeper emitter on exposed structures.
236 Sven Germershausen et al. / Energy Procedia 8 (2011) 232–237
Fig. 4 (a) Laser doped 82 Ohm/sq (3.4 J/cm²) emitter (relatively homogenous); (b) 34 Ohm/sq (3.8 J/cm²) emitter (not homogenous); (c) 17 Ohm/sq (4.2 J/cm²) emitter (strong inhomogeneous) on mono crystalline silicon 
By using ECV measurement, the measured val
Click here to load reader